This article has Open Peer Review reports available.
In vivo wear performance of highly cross-linked polyethylene vs. yttria stabilized zirconia and alumina stabilized zirconia at a mean seven-year follow-up
© Hasegawa and Sudo; licensee BioMed Central Ltd. 2013
Received: 30 July 2012
Accepted: 23 April 2013
Published: 1 May 2013
Zirconia was introduced as an alternative to alumina for use in the femoral head. The yttria stabilized zirconia material was improved by adding alumina. We evaluated highly cross-linked polyethylene wear performance of zirconia in total hip arthroplasty. The hypothesis was that alumina stabilized zirconia could decrease highly cross-linked polyethylene wear.
Highly cross-linked polyethylene wear was measured with a computerized method (PolyWare) in 91 hips. The steady-state wear rates were measured based on the radiographs from the first year postoperatively to the final follow-up and were compared between hips with yttria stabilized zirconia and alumina stabilized zirconia.
The steady-state wear rate of highly cross-linked polyethylene against zirconia was 0.02 mm/year at a mean follow-up of 7 years. No significant difference was observed between groups with yttria stabilized zirconia and alumina stabilized zirconia.
Addition of alumina to the zirconia material failed to show further reduction of highly cross-linked polyethylene wear and our hypothesis was not verified.
Polyethylene wear debris is a known cause of osteolysis and loosening in total hip arthroplasty (THA). Femoral heads with improved surface characteristics have been introduced to reduce the wear. In an attempt to reduce polyethylene wear, ceramic femoral heads have been used as an alternative bearing surface. Alumina ceramic was first introduced as a ceramic material for femoral heads. Alumina ceramic has excellent geometric form and wettable surface, enhances hardness, thereby maintaining lubrication, and increases resistance to third-body wear . Despite the excellent wear characteristics of alumina ceramic, a historic problem has been that, under certain conditions, it is prone to fracture .
Zirconia ceramic was introduced in 1985 as an alternative to alumina ceramic for the femoral head. Zirconia is tougher and more resistant to fracture [3, 4]. Zirconia ceramic has three phases of physical structure. The tetragonal phase has the greatest toughness and is used for the manufacture of prosthetic femoral heads, but it is also the most unstable phase with possible surface transformation back into the more stable monoclinic phase [5, 6]. Alloying pure zirconia with stabilizing oxides such as MgO and Y2O3 allows the retention of the tetragonal structure at room temperature . Yttria-stabilized tetragonal zirconia polycrystal (Y-TZP) has been used extensively. However, with Y-TZP, the potential exists for late phase transformation and aging, resulting in grain pullout, surface cracking, and increasing surface roughness . In one study of 52 retrieved Y-TZP heads, the monoclinic content within the bearing surface averaged 40% compared with 3% in nonimplanted heads [8, 9]. The tetragonal to monoclinic phase transformation of zirconia can be suppressed by the addition of a small amount of aluminum oxide (Al2O3). Recent improvements achieved by the addition of 0.25 wt% of Al2O3 have increased the static and dynamic fracture strengths of zirconia, giving higher resistance to low-temperature aging degradation and phase transformation . On the other hand, highly cross-linked polyethylene has been shown to achieve wear reduction compared with conventional polyethylene using a hip simulator . Several clinical studies have also shown improved wear rates for highly cross-linked polyethylene cups compared with conventional polyethylene cups against cobalt-chromium heads in midterm follow-up [12–14]. If ceramic heads and highly cross-linked polyethylene cups were coupled, further reductions in polyethylene wear could be expected. A few studies examined the clinical efficacy of this combination of highly cross-linked polyethylene cup with a zirconia head [13, 15–17]. However, no reports have yet examined the influence of improvement of the material for polyethylene wear. The purpose of this study was to evaluate the clinical outcomes and in vivo polyethylene wear performance of yttrium-oxide-partially-stabilized zirconia (PSZ) and alumina stabilized zirconia (ASZ) after a minimum 5-year follow-up. Both zirconia (PSZ and ASZ) were manufactured by Japan Medical Materials Corp. (JMM, Osaka, Japan). The hypothesis was that ASZ could decrease wear of highly cross-linked polyethylene. Retrieved PSZ and ASZ heads from this cohort of patients were also compared to never-implanted heads.
Demographic characteristics of two groups
Number of Hips
Body Mass Index (kg/m2)
Polyethylene Thickness (mm)
The cementless cup consisted of a titanium alloy metal shell (QPOC; JMM, Osaka, Japan) and a highly cross-linked ultra–high-molecular-weight polyethylene shell (Excellink; JMM, Osaka, Japan). The surface of the metal shell was porous-coated with pure titanium and a coating of apatite-wollastonite (AW) glass-ceramic was applied to the porous area. The metal shell was fixed with titanium screws to ensure primary fixation. The highly cross-linked polyethylene shell was gamma-irradiated to 50 kGy, heat annealed, and sterilized with 25 kGy of gamma radiation in nitrogen. The stem was a HS-6 collarless stem made of titanium alloy and was proximally porous-coated with an AW glass-ceramic. The head was a 26-mm yttria-stabilized zirconia head secured with a Morse taper. Improvements have been achieved by the addition of 0.25 wt% of Al2O3 (ASZ) since 2002.
Four patients (5 hips) died from unrelated medical conditions within 5 years after the THA and one patient was lost to follow-up. Three patients (3 hips) underwent revision due to infection (1 hip) and recurrent dislocation (2 hips) within 5 years after the THA. Thirteen patents (17 hips) underwent clinical evaluation without radiographs in our institution after a minimum follow-up of 5 years. After excluding those patients, 79 patients (91 hips) underwent both clinical and radiographic evaluations after a minimum follow-up of 5 years (mean, 7 years; range, 5–9.2 years). Sixty-eight hips received an improved zirconia head. Demographic characteristics of two groups are shown in Table 1. Full weight bearing was allowed 5 days postoperatively. Clinical and radiographic evaluations were scheduled immediately, after 6 weeks, 3 months, 6 months, and 1 year, and then annually after surgery. This study was approved by the institutional review board of Mie University Hospital, and all patients gave informed consent for the report to be published.
Clinical evaluation was performed using the Merle d’Aubigné and Postel scoring system . We assessed the score before primary arthroplasty and at the last follow-up. At each follow-up, standardized anteroposterior and lateral radiography of the hip was performed without weight-bearing. Anteroposterior radiographs were taken of bilateral hip joints with the patient in a supine position. Serial radiographs were analyzed by the same independent observer (M.H.). We used three radiographs per patient to determine the polyethylene wear. We selected the 3-week postoperative radiograph as a baseline. In addition, we analyzed the 1-year and last follow-up radiographs. We performed radiographic measurements of two-dimensional femoral head penetration into the polyethylene with a computerized method (PolyWare 5.10 digital version; Draftware Developers Inc., Vevay, IN) validated for clinical measurement of polyethylene wear in metal-backed acetabular components . Linear wear was measured in the plane of the anteroposterior radiograph by the software with an accuracy of 0.022 mm [19, 20]. Penetration of the femoral head into the acetabular polyethylene is due to a combination of creep and wear. The total head penetration rate was calculated based on the latest follow-up radiographs by dividing the observed head penetration by the postoperative period. Because creep deformity could be gained until about 1 year postoperatively [12, 13], the steady-state wear rates were measured based on the radiographs from the first year postoperatively to the final follow-up. Radiographic loosening of the acetabular component was evaluated using the method of Hodgkinson et al. . Radiographic loosening of the femoral component was evaluated using the method of Engh et al. . The inclination of the cup was measured. We compared the polyethylene wear between PSZ and ASZ. The effects of several factors on wear rates were examined, including sex, age, body mass index, liner thickness, cup inclination, and postoperative Merle d’Aubigné and Postel score .
Three zirconia femoral heads, retrieved at the time of revision procedures due to infection and recurrent dislocation, were analyzed to determine the surface roughness (Ra) using a contact surface profilometer (SV-3100; Mitutoyo Corporation, Kawasaki, Japan). The parameter Ra was the mathematical average of all deviations (peaks and valleys) from the mean line of the surface profile. The monoclinic content of the surface of the zirconia head was calculated with x-ray diffraction (PW3050; Spectris Co. Ltd., Tokyo, Japan). Scanning electron microscopy was used to evaluate the topography of the retrieval surfaces. The durations of implantation of these three zirconia femoral heads were 1.5, 2.3, and 3.2 years. Two unused zirconia heads were also examined. One head did not contain alumina (PSZ) and the other head contained alumina (ASZ).
Statistical analysis was performed using the Wilcoxon signed rank test and the Mann–Whitney U test for continuous variables. The chi-squared test and Fisher’s exact test was used for categorical data. Correlation analysis was performed using Spearman’s rank correlation test. A multiple regression test was also used. Statistical significance was set at p < 0.05. Kaplan-Meier survivorship for the entire population of 117 hips was analyzed with revision as the endpoint in 100 patients.
Osteolysis was not found around the implant and no zirconia head had a fracture. No hip showed findings of aseptic loosening; however, one hip showed acetabular loosening because of late infection. Postoperative dislocation occurred in five hips. Three patients (three hips) underwent revision from 1.5 to 3.2 years after the initial operation. Of these, one hip underwent a revision because of infection with acetabular loosening. In two patients, the components were revised because of recurrent dislocation. The clinical results of the 79 patients (91 hips) revealed that the mean Merle d’Aubigné and Postel score for this group had improved significantly from 9.6 points (range, 2 to 16) preoperatively to 15.3 (range, 7 to 18) (p < 0.001) postoperatively. The mean scores for pain, mobility, and walking ability improved from 2.8 (range, 0 to 5), 4.4 (range, 0 to 6), and 2.3 (range, 0 to 6) preoperatively to 5.6 (range, 3 to 6), 5.5 (range, 2 to 6), and 4.3 (range, 0 to 6) at the last follow-up, respectively.
Transformation rate and surface roughness of retrieved and unused zirconia heads
Cause of Revision
Transformation rate (%)
Surface roughness Ra (μm)
The addition of alumina to the zirconia material contributed to the reduced transformation rate; however, further reduction of highly cross-linked polyethylene wear was not achieved.
Summary of maximum transformation rate and surface roughness of retrieved yttria stabilized zirconia heads
Comparison of polyethylene wear against yttria stabilized zirconia, cobalt chromium, and alumina heads
Penetration Rate (mm/year)
Yttria Stabilized Zirconia
Stilling et al. 
Cohn et al. 
Kraay et al. 
Nakahara et al. 
Hernigou et al. 
Liang et al. 
Summary of highly cross-linked polyethylene wear against yttria stabilized zirconia heads
Steady-state wear rate
Yttria stabilized zirconia
Nakahara et al. 
Kawate et al. 
Fukui et al. 
Miyanishi et al. 
The present study failed to show further reduction of highly cross-linked polyethylene wear using the new zirconia. The mean age of the patients with the new zirconia was 57 years as opposed to 64 years in the patients with PSZ. Since patients are usually more active when they are younger, it is not fair to conclude that the newer-style heads did not contribute to lower wear. Hernigou and Bahrami  showed that the increase in rate of conventional polyethylene wear against Y-TZP head was only evident after eight years and might be linked to a long-term biodegradation of zirconia in vivo. Comparing new head with old head in the early years, the wear may be similar, but as time goes on we might see a difference in this cohort. Long-term wear studies are warranted. This study has some limitations. First, the small number of retrieval heads was studied. Second, this study has no comparison with cobalt-chromium heads. Third, the mean apparent measured steady-state wear rates (0.02 mm/year) were actually lower than the accuracy threshold of our method (0.022 mm).
The steady-state wear rate of highly cross-linked polyethylene against PSZ and ASZ heads were very low. No mechanical failures of the polyethylene or zirconia occurred. While our numbers were insufficient to compare degradation of material, addition of alumina to the zirconia material (ASZ) contributed to a reduction in the transformation rate; however, further reduction of highly cross-linked polyethylene wear was not achieved and our hypothesis was not verified.
There are no acknowledgements and no funding was obtained for this study.
- Sedel L, Nizard RS, Kerboull L, Witvoet J: Alumina-alumina hip replacement in patients younger than 50 years old. Clin Orthop Relat Res. 1994, 298: 175-183.PubMedGoogle Scholar
- Hasegawa M, Sudo A, Uchida A: Alumina ceramic-on-ceramic total hip replacement with a layered acetabular component. J Bone Joint Surg Br. 2006, 88: 877-882.View ArticlePubMedGoogle Scholar
- Christel P, Meunier A, Heller M, Torre JP, Peille CN: Mechanical properties and short-term in-vivo evaluation of yttrium-oxide-partially-stabilized zirconia. J Biomed Mater Res. 1989, 23: 45-61.View ArticlePubMedGoogle Scholar
- Kim YH: Comparison of polyethylene wear associated with cobalt-chromium and zirconia heads after total hip replacement. A prospective, randomized study. J Bone Joint Surg Am. 2005, 87: 1769-1776.View ArticlePubMedGoogle Scholar
- Hamadouche M, Sedel L: Ceramics in orthopaedics. J Bone Joint Surg Br. 2000, 82: 1095-1099.View ArticlePubMedGoogle Scholar
- Lawson S: Environmental degradation of zirconia ceramics. J Eur Ceram Soc. 1995, 15: 485-502.View ArticleGoogle Scholar
- Denry I, Kelly JR: State of the art of zirconia for dental applications. Dent Mater. 2008, 24: 299-307.View ArticlePubMedGoogle Scholar
- Fernandez-Fairen M, Blanco A, Murcia A, Sevilla P, Gil FJ: Aging of retrieved zirconia femoral heads. Clin Orthop Relat Res. 2007, 462: 122-129.View ArticlePubMedGoogle Scholar
- Cohn RM, González Della Valle A, Peterson M, Cornell CN: Similar wear in total hip arthroplasties with metallic or zirconia femoral heads. HSS J. 2008, 4: 107-111.View ArticlePubMedPubMed CentralGoogle Scholar
- Liang B, Kawanabe K, Ise K, Iida H, Nakamura T: Polyethylene wear against alumina and zirconia heads in cemented total hip arthroplasty. J Arthroplasty. 2007, 22: 251-257.View ArticlePubMedGoogle Scholar
- Muratoglu OK, Bragdon CR, O’Connor DO, Jasty M, Harris WH: A novel method of cross-linking UHMWPE to improve wear, reduce oxidation, and retain mechanical properties. J Arthroplasty. 2001, 16: 149-160.View ArticlePubMedGoogle Scholar
- Bragdon CR, Barrett S, Martell JM, Greene ME, Malchau H, Harris WH: Steady-state penetration rates of electron beam-irradiated, highly cross-linked polyethylene at an average 45-month follow-up. J Arthroplasty. 2006, 21: 935-943.View ArticlePubMedGoogle Scholar
- Nakahara I, Nakamura N, Nishii T, Miki H, Sakai T, Sugano N: Minimum five-year follow-up wear measurement of longevity highly cross-linked polyethylene cup against cobalt-chromium or zirconia heads. J Arthroplasty. 2010, 25: 1182-1187.View ArticlePubMedGoogle Scholar
- Mu Z, Tian J, Wu T, Yang J, Pei F: A systematic review of radiological outcomes of highly cross-linked polyethylene versus conventional polyethylene in total hip arthroplasty. Int Orthop. 2009, 33: 599-604.View ArticlePubMedPubMed CentralGoogle Scholar
- Miyanishi K, Hara T, Kaminomachi S, Maekawa M, Iwamoto M, Torisu T: Short-term wear of Japanese highly cross-linked polyethylene in cementless THA. Arch Orthop Trauma Surg. 2008, 128: 995-1000.View ArticlePubMedGoogle Scholar
- Kawate K, Ohmura T, Kawahara I, Tamai K, Ueha T, Takemura K: Differences in highly cross-linked polyethylene wear between zirconia and cobalt-chromium femoral heads in Japanese patients: a prospective, randomized study. J Arthroplasty. 2009, 24: 1221-1224.View ArticlePubMedGoogle Scholar
- Fukui K, Kaneuji A, Sugimori T, Ichiseki T, Kitamura K, Matsumoto T: Wear comparison between a highly cross-linked polyethylene and conventional polyethylene against a zirconia femoral head: minimum 5-year follow-up. J Arthroplasty. 2011, 26: 45-49.View ArticlePubMedGoogle Scholar
- Postel M, Merle d’Aubigné R: Functional results of hip arthroplasty with acrylic prosthesis. J Bone Joint Surg Am. 1954, 36: 451-475.PubMedGoogle Scholar
- Devane PA, Horne JG: Assessment of polyethylene wear in total hip replacement. Clin Orthop Relat Res. 1999, 369: 59-72.View ArticlePubMedGoogle Scholar
- Stilling M, Nielsen KA, Søballe K, Rahbek O: Clinical comparison of polyethylene wear with zirconia or cobalt-chromium femoral heads. Clin Orthop Relat Res. 2009, 467: 2644-2650.View ArticlePubMedPubMed CentralGoogle Scholar
- Hodgkinson JP, Shelley P, Wroblewski BM: The correlation between the roentgenographic appearance and operative findings at the bone-cement junction of the socket in Charnley low friction arthroplasties. Clin Orthop Relat Res. 1988, 228: 105-109.PubMedGoogle Scholar
- Engh CA, Bobyn JD, Glassman AH: Porous-coated hip replacement: the factors governing bone ingrowth, stress shielding, and clinical results. J Bone Joint Surg Br. 1987, 69: 45-55.PubMedGoogle Scholar
- Roy ME, Whiteside LA, Katerberg BJ, Steiger JA, Nayfeh T: Not all zirconia femoral heads degrade in vivo. Clin Orthop Relat Res. 2007, 465: 220-226.PubMedGoogle Scholar
- Hayaishi Y, Miki H, Yoshikawa H, Sugano N: Phase transformation of a new generation yttria-stabilized zirconia femoral head after total hip arthroplasty. Mod Rheumatol. 2008, 18: 647-650.View ArticlePubMedGoogle Scholar
- Brown SS, Green DD, Pezzotti G, Donaldson TK, Clarke IC: Possible triggers for phase transformation in zirconia hip balls. J Biomed Mater Res B Appl Biomater. 2008, 85: 444-452.View ArticlePubMedGoogle Scholar
- Hernigou P, Bahrami T: Zirconia and alumina ceramics in comparison with stainless-steel heads. Polyethylene wear after a minimum ten-year follow-up. J Bone Joint Surg Br. 2003, 85: 504-509.View ArticlePubMedGoogle Scholar
- Haraguchi K, Sugano N, Nishii T, Miki H, Oka K, Yoshikawa H: Phase transformation of a zirconia ceramic head after total hip arthroplasty. J Bone Joint Surg Br. 2001, 83: 996-1000.View ArticlePubMedGoogle Scholar
- Santos EM, Vohra S, Catledge SA, McClenny MD, Lemons J, Moore KD: Examination of surface and material properties of explanted zirconia femoral heads. J Arthroplasty. 2004, 19 (7 Suppl 2): 30-34.View ArticlePubMedGoogle Scholar
- Kim YH, Ritchie A, Hardaker C: Surface roughness of ceramic femoral heads after in vivo transfer of metal: correlation to polyethylene wear. J Bone Joint Surg Am. 2005, 87: 577-582.PubMedGoogle Scholar
- Masonis JL, Bourne RB, Ries MD, McCalden RW, Salehi A, Kelman DC: Zirconia femoral head fractures: a clinical and retrieval analysis. J Arthroplasty. 2004, 19: 898-905.View ArticlePubMedGoogle Scholar
- Kraay MJ, Thomas RD, Rimnac CM, Fitzgerald SJ, Goldberg VM: Zirconia versus Co-Cr femoral heads in total hip arthroplasty: early assessment of wear. Clin Orthop Relat Res. 2006, 453: 86-90.View ArticlePubMedGoogle Scholar
- Clarke IC, Manaka M, Green DD: Current status of zirconia used in total hip implants. J Bone Joint Surg Am. 2003, 85 (Suppl 4): 73-84.PubMedGoogle Scholar
- Maccauro G, Piconi C, Burger W: Fracture of a Y-TZP ceramic femoral head. Analysis of a fault. J Bone Joint Surg Br. 2004, 86: 1192-1196.View ArticlePubMedGoogle Scholar
- The pre-publication history for this paper can be accessed here:http://www.biomedcentral.com/1471-2474/14/154/prepub
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.